Natural Rubber Latex and Gum Arabic: A Comparison of Physico-Chemical Properties

Physicochemical characterization of gums is an suitability for industrial application. This focus of this study is to determine the physio-ISSN: Abstract The present investigation deals with the determination of the physio-chemical properties of two commercial grade samples of local gums (Gum Arabic and Natural Rubber Latex (NRL)). The results revealed that the gum samples have high melting point that indicate thermal stability at room and moderate temperatures. The gum samples have about 95 % carbohydrate content and a corresponding high internal energy and can serve as a source of energy. The rheology of the samples revealed shear-thickening characteristics with gum Arabic being thixotropic and pseudo-plastic in nature while NRL was observed to be anti-thixotropic and rheopectic. Further results from the moisture absorption, contact angle and Fourier Transform Infrared Radioscopy (FTIR) analyses gave better insight into their hydroscopic behaviours. Gum Arabic has excellent water absorption capacity with less wettability as it consists mainly of more water-soluble compounds in comparison to Natural Rubber Latex. These insights from the study will enhance wider application of the gums with increased value-addition to the gums and the communities where they (can) thrive.


Introduction
Rubber latex and gum Arabic are gums which are water-soluble polysaccharides that are extractable land plants. They also contain some protein materials and are important agro-forestry resources in Nigeria [1]. They can enhance the viscosity and gelling ability with their dispersions. Hence, the key qualities of the gums are their water solubility and high viscosity in aqueous dispersions. Guar gums are harvested from the stems and branches of the resource gum trees as dry exudates. Hydrophobic affinity chromatography showed that gum Arabic is made up of three major constituents namely, Arabinogalactan (AG), Arabinogalactan protein (AGP), and Glycoprotein (GP). The highly branched polysaccharide part of the gum represents about 90% of the total gum [2]. The complex nature of plant gums is since each gum sample possess a special combination of sugar (monosaccharide unit) to form the polysaccharide. The most widely distributed sugar in plant gums are mannose, galactose, ramose, fructose, xylose, and the sugar acid. They contain residual amount of fats, protein, metabolites, metal ions, crude fibres etc. Raw materials of plant origin have proven to be relatively non-toxic, bio-compatible, readily accessible, economical, and cost effective. In this regard plant gums are used for wide industrial applications such as in the cosmetic, pharmaceuticals and in food industries [3].
The prediction of the properties of these gums is a challenge because of their heterogeneity in addition to their complex nature.
Hence, their industrial applications require reliable information that can only be obtained from proper characterization of samples. The physicochemical properties of a compound are the measurable physical and chemical characteristics by which the compound may interact with other systems. This characteristic collectively determines the quality, applicability or the end-use of the compound. In plant gums, these properties are directly influenced by the botanical type, age, location, nature of the growing soil and the climatic condition around the resource gum tree [1]. Physicochemical characterization of gums therefore is chemical properties and characterization of natural lubber latex and guar gum as found in Nigeria. This is to enable us gain insight into their quality, applicability, and end use in industries.  Formalin was added to the gum Arabic clear solution to prevent deterioration, and then stored [1] . Natural Rubber Latex: 300 ml of the crude rubber latex gum was tapped from the stem of rubber latex plant (hevea brasiliensis) using a v-shaped knife. The raw latex was then centrifuged to remove water molecules. Ammonia solution was then added to the solution to prevent deterioration [4].

Density and Specific Gravity Measurement
Density and specific gravity analysis of 1% w/v of the test samples was carried out using a density bottle and following methods described elsewhere [5]. The weight of the empty bottle was measured (W) using CWS Series weighing balance (accuracy of ±0.05% FS) and then weight of the bottle with 70ml of the test samples of gum acacia solution and rubber latex gum respectively as (W 1 ). The difference was taken to obtain the actual weight of the liquid solution; the weight was divided by the volume to obtain the density as shown in equation (1) 1 100 w w Density of the gum samples v Where, W 1 is the weight of bottle and the test sample of the gum solution, W is the weight of the empty bottle and V is the volume of the gum samples.

Ash Content and Moisture Content
The analysis of moisture and ash content was determined using 2 clean crucibles of known weight dried in an oven at 102 C for 30 minutes. 10g of both samples were placed in the crucibles and the put into an oven (Gallenkamp TM OV-420) at a regulated temperature of 125 C for 6 hours. The Moisture content was taken as percentage ratio of the change in the weight to the original sample weight. The dry weight of the ash was taken, and the ash was ignited at 550 C in a muffle furnace for 1 hour, content was cooled in a desiccator for 30 minutes and weighed. The ash content was taken as the percentage loss in weight after ignition to that of the original sample. Equation (2) and (3) gives the temperature for calculating % moisture and % ash content respectively.
Where; W 1 is the original weight of the gum samples, W 2 is weight of the gum samples after drying Where; C 1 is the dry weight of ash, C 2 is the weight of ash after ignition

Moisture Adsorption of the Dried Gum Samples
The gum samples were dried in an oven (Gallenkamp TM OV-420), then spread in a thin layer in a weighing dish and kept at 22 C and 42% relative humidity. The weight was measured at different times.

Volume 3 -Issue 1 Mod App Matrl Sci. pH Determination
The pH of 1% w/v of the gum samples solution was determined with a microprocessor-based pH meter (Jenway 3510) which was set to neutral at room temperature and the electrode was immersed into the solution.

Viscosity and Thixotropy Measurement
The viscosity and thixotropy of the samples were measured using a rheometer (Ostwald viscometer VS135, ±1.0% accuracy).
At room temperature of 25 C, the gum solution at a known concentration was poured from the bottle container into a 75ml beaker and the temperature measured using a thermometer. The speed of the viscometer was then adjusted to 0.5 rpm and the viscometer reading measured and recorded [6]. The procedure was repeated for different speeds and the readings taken.

Melting Point
A melting point capillary was used for this purpose. A tiny sample of the gum powder was placed on a piece of weighing paper. A few crystals of the gum powders were then placed in a thin walled capillary tube 10-15cm long, 1mm internal diameter, and closed at one end. The capillary, which contains the sample and the thermometer are then suspended so they can be heated slowly and evenly. The temperature at which the sample was observed to melt is taken as the melting point. This was performed for each of the gum Acacia and rubber latex sample [7].

Surface Tension by Contact Angle
Droplets of the samples was placed on a flat surface and the angle between the surface and the droplet surface with respect to air was measured using a modular "CAM 200 -optical contact angle and surface tension meter" at different time intervals.

Internal Energy
The energy value was calculated by the factors of 4, 9, 4. Here the value of the protein content was multiplied by 4, that of lipid by 9 and that of total carbohydrate by 4. The sum of these values was expressed in kcal/100g sample [8,1].

Water Absorption
This was performed following ASTM D570. The gum samples were dried in an oven for 6 hours at 125 C and then placed in a desiccator to cool. Immediately upon cooling the specimens were weighed. The materials were then immersed in water at 25 C for 10 hours. The specimens were removed and reweighed.

Fourier Transform Infrared Spectroscopy (FTIR) Analysis
FTIR is commonly used for qualitative identification of various functionalities; the FTIR spectrum of the gum samples was recorded with a Perkin Elmer RXI spectrophotometer. The gum samples were mixed with KBr (potassium bromine) and examined by infrared spectroscopy because these spectra are usually sensitive to chemical composition [8].  Guar gum is observed to have a melting temperature of 76 C which is far less than the value 295 C reported by [1]. This huge difference may be due to the level of D-galactose (heterogeneous nature) of the gum exudates, as gums of higher D-galactose have higher melting point [7]. The water adsorption capacity of NRL sample was strikingly low (14.53%) compared to guar gum (86.58%). It also suggests the presence of more hydrophilic sites/pores in guar gum. While guar gum contains salts that can form hydrates, NRL contains isoprenes and other unsaturated hydrocarbons that have hydrophobic properties and hence are insoluble in water. This may suggest why it is used for water shielding purposes as well as in other non-food industries for the fabrication of plastics, automobile tires, balls etc. Guar gum on the other hand finds application even in food additives [11] as well as other applications because of its solubility in water [11,6]. The higher amount of nitrogen and protein (amines) in guar gum further lends credence to the obtained pH that suggests the presence of ammonia and possession of alkaline properties [2].

Effect of Shear Rate on Viscosity and Thixotropy
The (Figures 1,2) respectively gives the variation of viscosity and thixotropy of the gum samples under shear. For both samples,

viscosity increases with shear rates howbeit in different proportion
The difference in the response of the viscosities to shear rate may be related to the D-galactose content. Both gums exhibited shearthickening properties with NRL exhibiting higher shear-thickening and rheopectic characteristics. Gum Arabic is seen to exhibit the property of a Bingham plastic and hence non-Newtonian due to its response to shear. The observations here slightly vary from those reported by Yusuf [1], and could be partly due to the D-galactose content. The viscosity of their solution is therefore influenced by the prevailing temperature [13].     It can be deduced that NRL promotes better wettability because its contact angle decreases rapidly with time, hence its bonding strength is enhanced with increase in effective surface area. This may also explain why Cobblers spread their gums so thinly on surfaces that needs to be joined. This property of wettability may be related to their poor water absorption characteristics as discussed in Table 1. The excellent water absorption capacity of gum Arabic implies that its wettability will be less as shown in (Figure 3).

Wettability and Contact Angle
Despite displaying good bonding characteristics i.e., it does not wet a surface easily, targeted modifications of the material will have to be undertaken to enhance and maximize the material's bonding properties. However, this property makes it an excellent stabilizing agent in many beverages (norevo.de, 2017).   with medium intensity at 1408.9 cm -1 and 1248.7 cm -1 . A stretch of strong intensity peak of the alkyl halide group was observed at (Farar kaya) and Acacia nilotica (Bagaruwa). The differences in the location of the functional groups may be related to tree origin and duration of harvest of the gum crystals. The presence of strong peaks of the alcoholic compounds, carboxylic acid and Alkyl halide may further explain the degree of solubility and water absorption capacity and wettability of gum Arabic. In the NRL spectra ( Figure   5), weak intensity Amine group (RR 'N-H) was observed at 3665.8 cm -1 , while the presence of Amide (R-C (O) -NR'R") of strong intensity was seen at 1636.3 cm -1 . At 1446.2 cm -1 , alkyl (CH 2 ) n bend of medium intensity was present and nitro-compounds (R-NO 2 ) at 1375.4 cm -1 with medium intensity, as well as strong intensity peaks of Ethers (Ar-O-R) at 1073.5 cm -1 . and it is close in agreement with that reported [14][15][16][17][18][19][20][21].

Conclusion
The following can be concluded from the results obtained from the study.
a. Gum samples have high densities with corresponding thermally stability.
b. Both gums are carbohydrates by composition with high internal energy content.
c. The viscosity of both samples increases with shear rate with gum Arabic displaying thixotropic and pseudo-plastic properties and NRL noted be anti-thixotropic and rheopectic. e. FTIR was shown to be a useful technique to discern the functional groups present in any organic material.